Contents lists available at ScienceDirect

Ultramicroscopy journal homepage: www.elsevier.com/locate/ultramic

Quantitative use of electron energy-loss spectroscopy Mo-M2,3 edges for the study of molybdenum oxides L. Lajaunie n,1, F. Boucher, R. Dessapt, P. Moreau Institut des Matériaux Jean Rouxel (IMN), Université de Nantes, CNRS, 2 rue de la Houssinière, BP 32229, 44322 Nantes Cedex 3, France

art ic l e i nf o

a b s t r a c t

Article history: Received 25 June 2014 Received in revised form 20 October 2014 Accepted 6 November 2014 Available online 11 November 2014

Because of the large energy separation between O-K and Mo-L2,3 edges, extracting precise and reliable chemical information from core-loss EELS analyze of molybdenum oxides has always been a challenge. In this regard Mo-M2,3 edges represents an interesting alternative as they are situated close to the O-K edges. They should allow thus the extraction of a wealth of chemical information from the same spectra. However the main difﬁculty to overcome in order to work properly with these edges is the delayed maxima of the Mo-M4,5 edges which hinders the automated background subtraction with the usual inverse power low function. In this study we propose another background subtraction method speciﬁcally designed to overcome this obstacle and we apply it to the study of MoO3 and MoO2. We are able to show that quantitative chemical information can be precisely and accurately determined from the joined analyze of O-K and Mo-M2,3 edges. In particular k-factors are derived as a function of the integration window width and standard errors close to 2% are reported. The possibility to discriminate the two oxides thanks to chemical shifts and energy-loss near-edge structures is also investigated and discussed. Furthermore the M3/M2 ratios are derived and are found to be strongly dependent on the local chemical environment. This result is conﬁrmed by multiplet calculations for which the crystal ﬁeld parameters have been determined by ab initio calculations. The whole methodology as well as the conclusions presented in this paper should be easily transposable to any transitions metal oxides of the 4d family. This work should open a new and easier way regarding the quantitative EELS analyses of these compounds. & 2014 Elsevier B.V. All rights reserved.

Keywords: MoO2 MoO3 Electron energy-loss spectroscopy (EELS) M2,3 edges Quantiﬁcation Valence state

1. Introduction In the last few years, a lot of attention and efforts were dedicated to the nanoengineering of molybdenum oxides with control of size and shape. This has triggered the efﬁcient and successful synthesis of an extraordinary variety of molybdenum oxide nanostructures with tunable morphologies including nanoplates, nanostars, nanowires, nanobelts, nanoﬂakes, comblike nanostructures, mesoporous nanowalls, nanorods and nanotubes [1–9]. Pioneering studies have shown that these nanostructures present enhanced physical and chemical properties when compared to their bulk counterparts and that they are promising candidates for a wide variety of technological and marketable applications including electronic and optoelectronic devices, gas-sensors, ﬁeldemitters, electrochemical supercapacitors and positive materials for Li-batteries [1,4,8,10–12]. This should open the way for an n

Corresponding author. E-mail address: [email protected] (L. Lajaunie). 1 Present address: Laboratorio de Microscopías Avanzadas (LMA), Instituto de Nanociencia de Aragón (INA), Universidad de Zaragoza, Campus Río Ebro C/ Mariano Esquillor s/n 50018 Zaragoza, Spain. http://dx.doi.org/10.1016/j.ultramic.2014.11.002 0304-3991/& 2014 Elsevier B.V. All rights reserved.

emerging ﬁeld of research aiming at the characterization, comprehension and optimization of the properties of molybdenumbased nanostructures and associated nanodevices. The next challenge lies thus in the development of appropriate experimental tools for their characterization considering that as a strong need in this direction is expected. One key parameter inﬂuencing the chemical and physical properties of these compounds is their oxygen content that should be determined accurately and with enough spatial resolution [10,13,14]. Electron energy-loss spectroscopy (EELS) performed in a transmission electron microscope (TEM) is a method of choice to perform quantitative chemical investigations at the nanoscale. Theoretical determination of the scattering cross-sections allow for the quantiﬁcation of relative chemical concentrations of two elements A and B via Eq. (1),[15]:

σ (α, β, ΔE) NA I (α, β, ΔE) = A × B σA(α, β, ΔE) NB IB(α, β, ΔE)

(1)

where Ni is the number of atoms per unit area, Ii the integrated core-loss intensity within an energy windows of width ΔE starting close to the energy threshold of the energy edge and si(α,β,ΔE) the partial ionization cross-section integrated over a collection

2

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

semi-angle β and corrected from the incident beam convergence semi-angle α. If the theoretical cross-sections are not known or not reliable, which is the case for Mo-M2,3 edges, the k-factor can be experimentally determined from a standard of known A–B composition via Eq. (2),[16] :

kAB =

σB(α, β, ΔE) I (α, β, ΔE) N = B × A σA(α, β, ΔE) IA(α, β, ΔE) NB

(2)

It is important to note that these k-factors are dependent on many intrinsic and extrinsic parameters (such as α, β, ΔE, and the methods used for background subtraction and multiple scattering deconvolution) and should be considered as a microscope and user dependent quantity. Generally speaking, EELS elemental quantiﬁcation is a time consuming and user intensive procedure, which cannot be excessively automated. Beyond elemental quantiﬁcation, many other quantitative and qualitative information can be deduced from a core-loss spectrum by studying, for instance, energy-loss near-edge structures (ELNES), integrated intensity ratios from L2,3 edges as well as chemical shifts. The detailed analysis of all these aspects is far beyond the scope of this paper and the interested reader may refer to a numerous literature on this subject [15,17–19]. If EELS quantiﬁcation is a well-established technique, quantitative EELS analysis of 4d transition metals (TM) oxides remains a challenge so far. The L2,3 edges of these TM oxides are situated at high-energies and cannot be used with conﬁdence because of the excessively long dwell times and therefore unavoidable irradiation beam damages. For instance, the Mo-L2,3 edges are located around 2500 eV and are too far away from the O-K edge (530 eV) to allow pertinent Mo valence determination and precise Mo/O elemental quantiﬁcation from the same spectrum. Compared to 3d-TM, the EELS literature on 4d-TM is thus scarce and focus mainly on the study of M4,5 edges (involving transitions of 3d electrons) which lies roughly between 150 and 300 eV. In 1987, Hofer has shown that M4,5 edges can be used for elemental quantiﬁcation of MoO3 by determining the k-factors [20], and the same method was applied more recently to quantify niobium oxides [21,22]. The main drawback of using 4d-TM-M4,5 edges lies however in the delayed maximum that hinders the precise determination of the edge offset and thus has a detrimental effect on the precision of the elemental quantiﬁcation. The presence of the C-K edge around 290 eV can also be an additional challenge in case of carbon contamination during the EELS experiment or study of carbon-contained materials. In order to overcome these difﬁculties, the 4d-TM-M2,3 edges (transitions involving electrons in 3p orbitals) represent an interesting alternative. They are situated ideally close to the O-K edge (around 430 eV for Mo-M2,3 edges for instance) and display sharp peaks similar to the L2,3 white-line edges of TM and rare-earth compounds. To date, these edges are widely ignored by the EELS community and this is likely due to the delayed maxima of the M4,5 edges (around 300 eV for Mo-M4,5 edges) that appears as a broad rounded shoulder (Fig. 1a) and which hinders the automated background subtraction with the usual inverse power low function (Fig. 1b). However, the proximity between the O-K and 4d-TM-M2,3 edges is of great interest as it allows to collect them together while keeping a low experimental dispersion and thus avoiding a detrimental broadening effect on the energy resolution. A complete EELS study (going from ELNES analysis to elemental quantiﬁcation and even determination of M3/M2 ratio) might thus be performed on the same spectrum in order to obtain a wealth of chemical information. To our knowledge, only one EELS study using O-K and Mo-M2,3 edges has been reported so far in which the k-factor was determined from MoO3 and was used for the elemental quantiﬁcation of an unknown sample [24]. However,

Fig. 1. (a) EELS spectra of a molybdenum oxide recorded with a dispersion of 0.30 eV/pixel to highlight the peaks position and shape of the Mo-M.4,5, Mo-M2,3 and O-K. edges and (b) EELS spectra of a molybdenum oxide recorded with a dispersion of 0.20 eV/pixel highlighting the improper use of exponential and inverse power law functions to model the background continuum before the Mo-M.2,3 edge onset.

the authors did not give any details about the method they used for the background subtraction and, more importantly, the precision and the accuracy of their results was not discussed. Up to now, a quantitative and systematic EELS study of molybdenum oxides by means of M2,3 edges is still missing. Due to the proximity of molybdenum with niobium in the periodic table, insights can also be gained from the EELS literature on niobium oxides [21,22,25]. For instance, Bach et al. modeled the background before the Nb-M2,3 edges by using “predominantly an exponential function” and, from this, were able to derive the k-factors; however with a greater imprecision than the one determined from M4,5 edges [21]. It is worth noting that, in the case of molybdenum oxides, an exponential function fails to model properly the background before the M2,3 edges onset (Fig. 1b). Other approaches based on interpolation method [23] were also tested and found inappropriate to properly model the background before Mo-M2,3 edges onset. Other studies, in which the background was simply not removed, have mainly focused on chemical shifts and O-K edge ELNES analyzes [22,25]. This might explain some inconsistency regarding a possible link between niobium valence states and M3/M2 intensity ratios. In this paper, we explore the quantitative chemical information that can be derived from MoO3 and MoO2 compounds thanks to the joined analyze of Mo-M2,3 and O-K edges. In Section 2, the whole methodology is discussed. In particular, we present a new

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

method to subtract the background, which is speciﬁcally designed to overcome the difﬁculties when working with 4d transition metal M2,3 edges. The details of the calculations based on density functional theory and multiplet approaches are also given. In Section 3, the results regarding the ELNES, chemical shifts, elemental quantiﬁcation and sensitivity of the M3/M2 ratios are presented and discussed. The method to subtract the background is validated by the great precision and accuracy of the results. Finally, this work gives a clear answer to the nature and the precision of the quantitative information that can be extracted by using these edges and when applying our new method for background subtraction.

2. Materials and methods 2.1. Materials and EELS acquisition parameters

α-MoO3, the thermodynamically stable phase of the molybdenum trioxide in ambient conditions, and MoO2 have been used in this study because they are well known simple molybdenum oxides which contain 4d-metal ions with well-deﬁned oxidation states ( þIV and þVI, for MoO2 and MoO3 respectively), and in distinct chemical environments. Molybdenum trioxide α-MoO3 is described in an orthorhombic unit cell (space group Pbnm) with the cell parameters a ¼3.9624(1) Å, b¼13.860(2) Å, c ¼3.6971(4) Å [26]. The layered material is composed of [MoO3] sheets stacked along the [010] direction, and which are held together by van der Waals interactions (Fig. 2a). In the structure, the MoVI ion is linked to three crystallographically equivalent oxygen atoms in a strongly distorted octahedral environment (Mo–O bond lengths in the 1.67–2.33 Å range). The [MoO6] octahedra are then condensed via edge and corner-sharing to give rise to the [MoO3] sheets. Molybdenum dioxide MoO2 has a rutile-like structure which is described in a monoclinic unit cell (space group P21/c) with the cell parameters a ¼5.6109(8) Å, b¼4.8562(6) Å, c¼ 5.6285(7) Å, β ¼ 120.95(1)° [27]. The MoIV ion is linked to two crystallographically equivalent oxygen atoms in an octahedral

Fig. 2. (a) Polyhedral representation of layered α-MoO.3: The [MoO3] sheets are built upon distorted [MoO6] octahedra linked together by edge- and corner-sharing (left). The layers are stacked along the b axis (right). (b) Polyhedral representation of the rutile-like structure of MoO2 (gold sphere: oxygen, blue octahedra: [MoO6]). (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

3

environment. The [MoO6] octahedra show very slight distortion (Mo–O bond lengths in the 1.97–2.07 Å range), and they are linked together by edge-sharing into inﬁnite [MoO4] chains running along the [100] direction (Fig. 2b). The chains are then condensed via corner-sharing into a three-dimensional MoO2 network. EELS spectra were acquired on commercial α-MoO3 and MoO2 powders using a Hitachi HF2000 TEM (100 kV) equipped with a cold ﬁeld emission gun and a modiﬁed Gatan PEELS 666 spectrometer. Experiments were performed at liquid nitrogen temperature to minimize carbon contamination and irradiation beam damage which are known to be important in MoO3 EELS experiments [24,28,29]. The acquisition time and the probe size for each core-loss were set to 20 s and 30 nm, respectively. The electron dose was measured in the same conditions with a Faraday cup and is equal to 2.7 106 e/nm2. The energy resolution, measured as the full width at half maximum (FWHM) of the zero loss peak (ZLP), was 1.5 eV with an energy dispersion of 0.20 eV/pixel. This dispersion allowed the recording of the Mo-M2,3 and O-K edges on the same spectra. Convergence and collection angle were 1.4 and 4.6 mrad, respectively. Thanks to this experimental setup (α/θE ¼0.7, β/θE ¼2.2 for an energy-loss of 400 eV with an acceleration voltage of 100 kV), EELS spectra were acquired at the magic angle condition for the Mo-M2,3 edges (βM/θE ¼ 2.25 for small αM/θE at 100 kV [30–33]) to avoid anisotropy effects playing a role in the determination of M3/M2 ratios. Each crystal was set slightly off zone axis to avoid channeling effects. At least 10 spectra per sample were acquired and processed to ensure the reproducibility of the results. 2.2. EELS data treatment All spectra were ﬁrst gain and dark count corrected and then deconvoluted by the ZLP using the PEELS program [34]. Background subtraction for the O-K edge was performed by modeling an inverse power law function I ¼A1E r1 in the pre-edge energy window 490–520 eV, where E represents the energy loss and where both A1 and r1 are constants. The extrapolated background was then subtracted as illustrated in Fig. 3a. Starting from the M3 edge onset ( 389 eV) the background was modeled by using an inverse power law function I ¼A2E r1 where the r1 parameter is the same than the one determined for the O-K edge. The main objective of this method is to avoid the detrimental effect of the Mo-M4,5 edges on the background subtraction. In addition, before the Mo-M3 edge onset, the background was modeled by using an exponential function (aebE, where a and b are constants) for the sole purpose to have a pre-edge qualitative indicator of the signal/ noise ratio. In order to reach convergence in an efﬁcient manner, these two ﬁts were achieved by using speciﬁc routines based on Nelder–Mead algorithms (unconstrained nonlinear optimization) [35]. The multiple scattering was then removed by Fourier-ratio deconvolution with the low-loss spectrum obtained for exactly the same region of the sample [15]. The resulting spectrum is displayed in Fig. 3b. In addition, the theoretical cross-section of Mo-L2,3 edges was calculated by using the parameterization of the generalized oscillator strength [15] thanks to the PEELS program [34]. For this purpose, the cross-section was calculated by constraining the maxima of the Mo-L2,3 edges to be close to the experimental maxima of the Mo-M2,3 edges. The tail of this calculated cross-section is displayed in Fig. 3b. As it can clearly be seen from this ﬁgure, there is an excellent agreement between the tails of the cross-section and the tail of the M2,3 edges after background and multiple scattering removal. This demonstrates that the method used to remove the background allows to recover an absorption edge which decreases in a coherent manner with what

4

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

Fig. 4. Method used for the determination of the M3/M2 ratios. A two-steps. function was subtracted and the ratios were determined by integration of the areas under the peaks.

respectively (Fig. 4). A great care was taken to check that no correlation exists between the experimental M3/M2 intensity ratios and the corresponding relative thicknesses (deduced from lowloss spectra) to rule out an improper multiple scattering deconvolution and/or the inﬂuence of irradiation beam damages [38]. 2.3. Multiplet and ab initio calculations

Fig. 3. (a) Method proposed in this paper to model the background continuum before the Mo-M2,3 edge onset and (b) the extracted spectrum after multiple scattering removal (thick black) and the tail of the cross-section of Mo-L2,3 edges computed around 400 eV (thin green). (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

would be expected in similar conditions of incident beam energy, energy position and collection and convergence angles. To determine the feasibility of elemental quantiﬁcation when using Mo-M2,3 edges, the k-factors kMoO were determined from MoO3 and MoO2 samples according to Eq. (2). The width of the energy windows (ΔE) was varied from 5 to 60 eV (by step of 5 eV) to check on the inﬂuence of this parameter on the quantiﬁcation results. Due to the low energy dispersion, larger energy window than 60 eV could not be achieved. To determine the M3/M2 intensity ratios, the maximum of the M3 edges were ﬁrst aligned to the same energy-loss (398 eV) to minimize the systematic error from peak positions and shapes. Following closely the work of Daulton and Little [36], a two-steps “zero-slope” function with the step onsets occurring at the white-line maximums was build and was further convoluted by a Gaussian function with a FWHM of 1.5 eV to match the experimental resolution. According to the authors, the “zero-slope” method yields less scattered results than the method used for instance by Pearson et al. [37], in which the slope follows the decrease of the cross-section of the considered edges. The ratio of the steps heights was set as 2:1 to reﬂect the multiplicity of the 3p1/2 and 3p3/2 initial states and the intensity function was adjusted to match the minimum intensity of the experimental spectrum between 420 and 425 eV. The two-steps function was then subtracted from the experimental spectra and the M3/M2 intensity ratios were determined by area integration from 399 to 407 eV and 407 to 423 eV for the M3 and M2 edges,

In order to check on the accuracy of the method proposed in this paper, experimental intensity ratios were also compared to theoretical one derived from multiplet calculations by using the CTM4XAS program [39]. Calculations were performed by reducing Slater integrals to 80% of their calculated atomic values. A 0.5 eV Lorentzian broadening was added to take into account life-time broadening and a 1.5 eV Gaussian broadening was also added corresponding to the experimental energy resolution. The crystal ﬁeld parameters (10 Dq), which were found to strongly affect calculated intensity M3/M2 ratios, were obtained from ab initio calculations based on the Density Functional Theory [40]. For this purpose, the ground-state electronic structures of α-MoO3 an MoO2 were determined with the all electron code WIEN2k [41] in the Perdew–Burke–Ernzerhof parameterization of the generalized gradient approximation (PBE-GGA). The structural data of α-MoO3 and MoO2 were taken from the work of Lajaunie et al. and Bolzan et al., respectively [42,43]. Mufﬁn-tin radii (RMT) were set to 1.96 Bohr radius for Mo and 1.7 Bohr radius for O. The self-consistencies on electronic density were obtained with a plane wave energy cutoff deﬁned by RMT KMAX ¼7 and by using (8 2 8) and (8 8 8) k-point meshes for MoO3 and MoO2, respectively. The 10 Dq were then determined from the band structures calculations by taking the average separation between the t2g and eg bands and were found to be equal to 3.5 eV for MoO3 and 4.5 eV for MoO2. Finally, theoretical M3/M2 ratios were derived from the calculated multiplet spectra by area integration in a similar manner than the one used for the experimental ratios.

3. Results and discussion 3.1. ELNES and chemical shifts Electron-energy-loss near edge structures (ELNES) originate from the electron transitions from core orbitals to unoccupied

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

bands. These spectral features can be envisaged in a ﬁrst-order approximation as an image of a momentum and atomic resolved projection of the unoccupied density of states. They are thus sensitive to the chemical bonding. Fig. 5a shows the ELNES of the O-K edge for MoO3 and MoO2. Both spectra are similar to those previously reported by EELS and XAS studies on the same compounds [24,44–49]. This shows that the dwell time of the EELS acquisition was set short enough to avoid the reduction of the samples under the electron beam as it was previously reported on molybdenum oxides [24]. Fig. 5a clearly shows that MoO3 and MoO2 can be distinguished thanks to the spectral shape of their O-K edges over an energy range of 10 eV above the absorption threshold. In particular, the O-K edge of MoO3 presents a ﬁrst strong peak (labeled A Fig. 5 a and with an absolute position of 531.270.3 eV) followed by two small shoulders (labeled B and C and situated around 532.5 eV and 534.5 eV, respectively) whereas MoO2 presents two peaks (labeled a and c in Fig. 5a and situated at 531.1 eV 7 0.5 and 534.5 70.4 eV, respectively) among which the second peak is the most intense. Going beyond this qualitative description would require a more complete experimental and theoretical study to link the O-K edge ﬁne structures of these two phases with their crystallographic structures as it have been done for other compounds [50]. Such study is still lacking even if previous studies on MoO3 and MoO2 interpreted the peaks near the absorption threshold as resulting from transitions of oxygen s core states to oxygen p states hybridized with the transitions metal t2g and eg states [40,49,51]. The ELNES of Mo-M2,3 edges for the two compounds are shown in

5

Fig. 5b. Except from a double-peak structure for the M3 edge of MoO3 (highlighted by an arrow in Fig. 5b) no clear spectral feature is distinguishable on the two spectra. The smallest features around the M2 edges are not reproducible and result from random noise rather than ﬁne-structures. It is worth noting that except a double peak-structure in the M2 edge of MoO3, XAS studies with considerably better energy resolutions (around 0.1–0.2 eV) do not reveal more speciﬁc features [49,52,53]. Absolute chemical shifts and energy differences can also be used as a ﬁngerprinting method to discriminate compounds with different oxidation states [15,19,54–56] although the measurement of absolute positions is quite tricky due to the TEM instabilities and often requires speciﬁc experimental setup or software during the data acquisition [19,57,58]. A better precision can generally be obtained by analyzing the difference in energy between two ELNES features. The question is thus to determine which ELNES quantity behaves most sensitively with a change of valence state. Table 1 presents the absolute position of the M3 maximum for the two oxides, the difference in energy between the two M edges maxima and ﬁnally, the difference in energy between the M3 maximum and the inﬂexion point of the O-K edge (determined by the change of sign of the second derivative). It is clear that MoO3 and MoO2 cannot be distinguished from the ﬁrst ELNES quantity, the average absolute position of the M3 maximum being identical. The same statement can be made for the second ELNES quantity since the difference falls in the error range. This is mostly due to the low signal/noise ratio around the M edges which hinders the precise determination of the M2 maximum. The measurements of the energy difference between the M3 maximum and the inﬂexion point of the O-K edge reveal a clear increase of 0.6 eV going from MoO3 to MoO2. With respect to the standard errors, this last result is statistically signiﬁcant. This evolution is consistent with the metallic and semiconductor nature of MoO2 and MoO3, respectively. More quantitative statements would however require comparison with calculations based on many-body approaches which are beyond the scope of this paper. In addition, the sensitivity of this ELNES quantity with this valence state is rather weak and other possibilities such as elemental quantiﬁcation and M3/M2 ratios are thus worth exploring. 3.2. Elemental quantiﬁcation and M3/M2 ratios One of the main purpose of this paper is to determine if a reproducible and accurate elemental quantiﬁcation can be achieved by using Mo-M2,3 and O-K edges. It is generally assumed that large energy windows should be avoided because they tend to maximize errors due to background extrapolation and thus compromise the precision of the quantiﬁcation. On the other hand, it is also advised to avoid small energy windows because of the differences of near-edge ﬁne structures which compromise the accuracy of the quantiﬁcation. To clarify this point, we have determined the k-factors and the corresponding standard deviation (95% conﬁdence interval) as a function of the energy width in Fig. 6. Except for the unreasonable energy window of 5 eV, all the values of kMoO are scattered close to 0.45 (Fig. 6a), thus showing that the partial cross-section obtained from the Mo-M2,3 edge is Table 1 Energy position of the maximum of the Mo-M3 edge, energy difference between the maxima of the Mo-M3 and Mo-M2 edges and energy difference between the maximum of the Mo-M3 edge and the inﬂexion point of the O-K edge.

Fig. 5. EELS spectra recorded on MoO3 and MoO2 samples showing the ELNES of the O-K edges (a) and Mo-M2,3 edges (b).

MoO3 MoO2

Mo-M3 (eV)

M3–M2 (eV)

Mo-M3–O-K (eV)

397.8 7 0.4 397.7 7 0.5

16.8 70.3 16.5 70.4

131.6 7 0.2 132.2 7 0.2

6

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

Fig. 7. Results of the quantiﬁcation for the MoO3 and MoO2 samples by using the average k-factors. The expected stoichiometries are given by the blue lines. (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

Fig. 6. (a) k-Factors for MoO3 (red squares) and MoO2 (black circles) determined from the Mo-M2,3 and O-K edges as a function of the energy window, ΔE. (b) Standard errors (95% conﬁdence interval) on the determination of the k-factors for MoO3 (red squares) and MoO2 (black circles) and relative difference to the mean deﬁned by (kMoO − k¯MoO)/k¯MoO (blue diamonds). (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

roughly twice as large as that obtained from the O-K edge. The standard errors are the highest for a width of 5 eV (around 15% and 10% for MoO3 and MoO2, respectively), reach a minimum close to 2% for energy windows of 15 and 20 eV for MoO2 and MoO3 respectively and, from there, increase slowly with the window width to reach a value around 4.5% for a width of 60 eV (Fig. 6b). Once averaged, the results obtained from the two compounds show a local minimum of the standard error for an energy window of 15 eV (kMoO ¼ 0.46 70.01 i.e., 2.2% of standard errors). Compared to literature, this result is more precise than that obtained from Bach et al. by using Nb-M2,3 edges on niobium oxides (7 7%) and presents a similar precision than their k-factors determined from Nb-M4,5 edges (72.1%) [21]. Olszta et al. determined the k-factors from the Nb-M4,5 edges solely and reached a precision slightly larger than 4% [22]. The precision and the accuracy of these results validate the method we used to subtract the background. In order to determine the accuracy of our results (and to check if the average values of the two k-factors can be used for quantiﬁcation), the relative difference to the mean is also plotted in Fig. 6.(b). This quantity is deﬁned as (kMoO − k¯MoO)/k¯MoO , where kMoO is the kfactor determined either from the MoO2 or the MoO3 sample and where k¯MoO is the mean value between the k-factors determined from the two samples. The relative difference to the mean presents strong variations depending on the energy window. The highest difference (14%) occurs with a width of 5 eV whereas the best accuracy (2%) on the determination of the k-factors is found for a width of 10 eV. A plateau with values around 4% is also found for

energy width of 15, 20 and 25 eV. To summarize and illustrate the effects of accuracy and precision of the quantiﬁcation, Fig. 7 shows the results of quantiﬁcation for the two samples by using the average k-factors. The standard errors on quantiﬁcation are evaluated by taking into account the errors on determination of the kfactors and integrated intensities. The highest accuracy is achieved with a 10 eV window width (NMo/NO ¼0.3370.03 (79%) and 0.517 0.04 ( 78%) for MoO3 and MoO2, respectively) whereas the highest precision is achieved with a 15 eV window width (NMo/NO ¼0.35 70.01 ( 73%) and 0.487 0.02 ( 74%) for MoO3 and MoO2, respectively). These two windows are thus the best choices for elemental quantiﬁcation and should be selected accordingly with the desired objective. Another interrogation remains concerning the sensitivity of the 4d-TM-M2,3 edges with the chemical environment of the metal. On this subject, contradictory results can be found in the EELS literature related to niobium oxides [22,25]. In particular, by using a variant of the Pearson’s method [37], Olszta et al. reported a correlation between the normalized white-line intensities and the 4d occupancy. However the authors did not discuss the accuracy of their method (in which the background subtraction before the Nb-M2,3 edges onset was not performed), and when applying the same method to MoO3 M2,3 edges, we ﬁnd a statistical error of nearly 30% on the sum of the white-line intensities. Due to the strong similarities between 4d-M2,3 and 3d-L2,3 edges related to their white-line nature (transitions from spin orbit split initial states to quasi-localized ﬁnal states), valuable insights can be gained again from the EELS and XAS literature related to 3d-L2,3 edges. The most popular and common EELS method to link the L2,3 edges with the chemical environment of a 3d-TM is without any doubt the L3/L2 integrated intensity ratio. This method is issued from the interrogations which were raised in the 80’s about the deviation between the experimental branching ratio and the statistical one (i.e. as expected from the degeneracy of the 2p states into 2p1/2 and 2p3/2 levels) [59–61]. Nowadays the origins of this deviation are still under investigation [62,63]. However it can be stated that the L3/L2 ratio is not only sensitive to the valence state of the metal [36,54] but rather to a complex mix between the local electronic structure of the cation, its local environment and, to some extent, bandstructure effects [64,65]. In this regard, this method is extremely interesting to track down subtle chemical changes on the local coordination but is extremely difﬁcult to

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

7

from MoO3 and MoO2, the same energy window yields an accuracy of 4%. This shows that Mo-M2,3 edges can be used for elemental quantiﬁcation with a precision equal or even better than those previously reported on 4d transition metal oxides with M4,5 edges. Furthermore the M3/M2 ratios can also be used to track down subtle chemical changes since they were found to be sensitive to the chemical environment of the 4d cation. In addition, the validity of the numbers extracted from the M3/M2 analysis was conﬁrmed by multiplet calculations. This work thus demonstrates the ability to obtain a wealth of precise and accurate chemical information on molybdenum oxides from the conjugated analyzes of O-K and Mo-M2,3 edges when the background is properly extracted thanks to the method proposed in this paper. It should also open interesting opportunities for the EELS studies of a large variety of materials as it is directly transposable to the whole family of 4d transition metal oxides. Fig. 8. Crystal ﬁeld multiplet calculation spectra for Mo6 þ (thick red line) and Mo4 þ (thin black line) calculated in octahedral environment. (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

interpret without multiplet and/or ab initio calculations and is thus generally used as a ﬁngerprinting method. Many variants of this method have been proposed and applied successfully on a large variety of compounds [18,19,29,36,54]. For MoO3 and MoO2, the experimental M3/M2 ratios were found to be equal to 1.91 70.05 (73%) and 2.20 70.04 ( 72%), respectively. Thanks to the method used for the background extraction, a high precision is found on the determination of the ratios. This result is of importance since it shows that the M3/M2 ratios are sensitive to the chemical environment of the 4d cation and that they can be used to make a clear distinction between the two oxides. In order to check on the validity of these numbers, the M3/M2 ratios were also determined from multiplet calculated spectra (Fig. 8) for which the crystal ﬁeld parameters have been previously estimated by DFT calculations. From a qualitative point of view, the calculated intensities match the intensities of the experimental spectra (Fig. 5b). For MoO3 and MoO2, the calculated M3/M2 ratios are equal to 1.99 and 2.26, respectively and are thus really close to the experimental ratios. This results assets our experimental methodology and it also implies that the “real” background under the M edges has been properly estimated.

4. Conclusion We have proposed another background subtraction method speciﬁcally designed to circumvent the difﬁculties arising when working with the M2,3 edges of the 4d transition metals oxides. This method was applied to MoO3 and MoO2 and allowed us to explore new possibilities given by the simultaneous analysis of O-K and Mo-M2,3 edges in term of ELNES differences, chemical shifts, elemental quantiﬁcation and M3/M2 ratio. Firstly, the two molybdenum oxides can be distinguished qualitatively thanks to the spectral shape of their O-K edges over an energy range of 10 eV. The difference in energy between the maximum of the M3 edge and the inﬂexion point can also be used since it was found to increase signiﬁcantly going from MoO3 to MoO2. Secondly, the M2,3 edges can be used for elemental quantiﬁcation and a great care was taken to determine the accuracy and precision of the kfactors as a function of the energy window used for the area integration. In particular, the best precision of the determination of k-factors is realized with an energy window of 15 eV and is close to 2%. Furthermore when comparing the k-factors determined

Ackowledgments We would like to thank Pr. F.M. De Groot for his help and discussion in the use of the CTM4XAS program.

References [1] T. Brezesinski, J. Wang, S.H. Tolbert, B. Dunn, Ordered mesoporous alpha-MoO3 with iso-oriented nanocrystalline walls for thin-ﬁlm pseudocapacitors, Nat. Mater. 9 (2010) 146–151. http://dx.doi.org/10.1038/NMAT2612. [2] D. Chen, M. Liu, L. Yin, T. Li, Z. Yang, X. Li, et al., Single-crystalline MoO3 nanoplates: topochemical synthesis and enhanced ethanol-sensing performance, J. Mater. Chem. 21 (2011) 9332–9342. [3] S. Hu, X. Wang, Single-walled MoO3 nanotubes, J. Am. Chem. Soc. 130 (2008) 8126–8127. [4] A. Khademi, R. Azimirad, A.A. Zavarian, A.Z. Moshfegh, Growth and ﬁeld emission study of molybdenum oxide nanostars, J. Phys. Chem. C 113 (2009) 19298–19304. [5] L. Mai, F. Yang, Y. Zhao, X. Xu, L. Xu, B. Hu, et al., Molybdenum oxide nanowires: synthesis & properties, Mater. Today 14 (2011) 346–353. [6] A. Okada, M. Yoshimura, K. Ueda, Fabrication of comblike nanostructures using self-assembled cluster arrays of molybdenum oxides, Appl. Phys. Lett. 90 (2007) 203102. [7] L.X. Song, J. Xia, Z. Dang, J. Yang, L.B. Wang, J. Chen, Formation, structure and physical properties of a series of alpha-MoO3 nanocrystals: from 3D to 1D and 2D, CrystEngComm 14 (2012) 2675–2682. http://dx.doi.org/10.1039/ c2ce06567c. [8] Z. Wang, S. Madhavi, X.W. (David) Lou, Ultralong alpha-MoO3 nanobelts: synthesis and effect of binder choice on their lithium storage properties, J. Phys. Chem. C 116 (2012) 12508–12513. http://dx.doi.org/10.1021/jp304216z. [9] B. Yan, Z. Zheng, J. Zhang, H. Gong, Z. Shen, W. Huang, et al., Orientation controllable growth of MoO3 nanoﬂakes: micro-Raman, ﬁeld emission, and birefringence properties, J. Phys. Chem. C 113 (2009) 20259–20263. [10] S. Balendhran, J. Deng, J.Z. Ou, S. Walia, J. Scott, J. Tang, et al., Enhanced charge carrier mobility in two-dimensional high dielectric molybdenum oxide, Adv. Mater. 25 (2013) 109–114. [11] N. Illyaskutty, S. Sreedhar, H. Kohler, R. Philip, V. Rajan, V.M. Pillai, ZnOmodiﬁed MoO3 nano-rods,-wires,-belts and-tubes: photophysical and nonlinear optical properties, J. Phys. Chem. C 117 (2013) 7818–7829. [12] P. Meduri, E. Clark, J.H. Kim, E. Dayalan, G.U. Sumanasekera, M.K. Sunkara, MoO3–x nanowire arrays as stable and high-capacity anodes for lithium ion batteries, Nano Lett. 12 (2012) 1784–1788. [13] I. Navas, R. Vinodkumar, V.P.M. Pillai, Self-assembly and photoluminescence of molybdenum oxide nanoparticles, Appl. Phys. Mater. Sci. Process. 103 (2011) 373–380. http://dx.doi.org/10.1007/s00339-011-6345-9. [14] F. Ferreira, T.G. Souza Cruz, M. Fantini, M. Tabacniks, S.C. de Castro, J. Morais, et al., Lithium insertion and electrochromism in polycrystalline molybdenum oxide ﬁlms, Solid State Ion. 136 (2000) 357–363. [15] R.F. Egerton, Electron Energy-loss Spectroscopy in the Electron Microscope, Springer Verlag, Berlin, 2011. [16] F. Hofer, G. Kothleitner, P. Rez, Ionization cross-sections for the L23-edges of the elements Sr to Mo for quantitative eels analysis, Ultramicroscopy 63 (1996) 239–245. [17] R. Brydson, A brief review of quantitative aspects of electron energy loss spectroscopy and imaging, Mater. Sci. Technol. 16 (2000) 1187–1198. [18] T. Riedl, T. Gemming, K. Wetzig, Extraction of EELS white-line intensities of manganese compounds: Methods, accuracy, and valence sensitivity, Ultramicroscopy 106 (2006) 284–291.

8

L. Lajaunie et al. / Ultramicroscopy 149 (2015) 1–8

[19] H. Tan, J. Verbeeck, A. Abakumov, G. Van Tendeloo, Oxidation state and chemical shift investigation in transition metal oxides by EELS, Ultramicroscopy 116 (2012) 24–33. [20] F. Hofer, EELS quantiﬁcation of M edges by using oxidic standards, Ultramicroscopy 21 (1987) 63–68. [21] D. Bach, H. Stormer, R. Schneider, D. Gerthsen, J. Verbeeck, EELS investigations of different niobium oxide phases, Microsc. Microanal. 12 (2006) 416–423. http://dx.doi.org/10.1017/S1431927606060521. [22] M.J. Olszta, J. Wang, E.C. Dickey, Stoichiometry and valence measurements of niobium oxides using electron energy-loss spectroscopy, J Microsc. 224 (2006) 233–241. http://dx.doi.org/10.1111/j.1365-2818.2006.01709.x. [23] R. Egerton, M. Malac, Improved background-ﬁtting algorithms for ionization edges in electron energy-loss spectra, Ultramicroscopy 92 (2002) 47–56. [24] D. Wang, D.S. Su, R. Schlogl, Electron beam induced transformation of MoO3 to MoO2 and a new phase MoO, Z. Anorg. Allg. Chem. 630 (2004) 1007–1014. http://dx.doi.org/10.1002/zaac.200400052. [25] R. Tao, R. Todorovic, J. Liu, R.J. Meyer, A. Arnold, W. Walkosz, et al., Electron energy-loss spectroscopy study of metallic Nb and Nb oxides, J. Appl. Phys. 110 (2011) 124313. [26] L. Kihlborg, Least squares reﬁnement of crystal structure of molybdenum trioxide, Ark. Kemi. 21 (1963) 357. [27] B.G. Brandt, A. Skapski, A reﬁnement of the crystal structure of molybdenum dioxide, Acta Chem. Scand. 21 (1967) 661–672. [28] D.E. Diaz-Droguett, A. Zuniga, G. Solorzano, V.M. Fuenzalida, Electron beaminduced structural transformations of MoO3 and MoO3 x crystalline nanostructures, J Nanopart. Res. 14 (2012) 679. http://dx.doi.org/10.1007/s11051011-0679-2. [29] Z. Wang, N. Dupré, L. Lajaunie, P. Moreau, J.F. Martin, L. Boutafa, et al., Effect of glutaric anhydride additive on the LiNi0.04Mn1.6O4 electrode/electrolyte interface evolution: a MAS NMR and TEM/EELS study, J. Power Sources 215 (2012) 170–178. [30] B. Jouffrey, P. Schattschneider, C. Hébert, The magic angle: a solved mystery, Ultramicroscopy 102 (2004) 61–66. [31] C. Hébert, P. Schattschneider, H. Franco, B. Jouffrey, ELNES at magic angle conditions, Ultramicroscopy 106 (2006) 1139–1143. [32] J.-C. Le Bossé, T. Epicier, B. Jouffrey, Polarization dependence in ELNES: inﬂuence of probe convergence, collector aperture and electron beam incidence angle, Ultramicroscopy 106 (2006) 449–460. [33] A. Sorini, J. Rehr, Z. Levine, Magic angle in electron energy loss spectra: relativistic and dielectric corrections, Phys. Rev. B 77 (2008) 115126. [34] P. Fallon, C.A. Walsh, PEELS Program, University of Cambridge, England, 1996 (PEELS Program Univ. Camb. Engl). [35] J.C. Lagarias, J.A. Reeds, M.H. Wright, P.E. Wright, Convergence properties of the Nelder–Mead simplex method in low dimensions, SIAM J. Optim 9 (1998) 112–147. [36] T.L. Daulton, B.J. Little, Determination of chromium valence over the range Cr (0)–Cr (VI) by electron energy loss spectroscopy, Ultramicroscopy 106 (2006) 561–573. [37] D. Pearson, C. Ahn, B. Fultz, White lines and D-electron occupancies for the 3d and 4d transition metals, Phys. Rev. B 47 (1993) 8471. [38] K.J. Livi, B. Lafferty, M. Zhu, S. Zhang, A.-C. Gaillot, D.L. Sparks, Electron energyloss safe-dose limits for manganese valence measurements in environmentally relevant manganese oxides, Environ. Sci. Technol. 46 (2011) 970–976. [39] E. Stavitski, F.M.F. de Groot, The CTM4XAS program for EELS and XAS spectral shape analysis of transition metal L edges, Micron 41 (2010) 687–694. http: //dx.doi.org/10.1016/j.micron.2010.06.005. [40] P. Moreau, F. Boucher, Revisiting lithium K and iron M-2, M-3 edge superimposition: the case of lithium battery material LiFePO4, Micron 43 (2012) 16–21. http://dx.doi.org/10.1016/j.micron.2011.05.008. [41] P. Blaha, K. Schwarz, G.K.H. Madsen, D. Kvasnicka, J. Luitz, WIEN2k, An Augmented Plane Waveþ Local Orbitals Program for Calculating Crystal Properties, Karlheinz Schwarz Techn Univ., Wien Austria., 2001. [42] L. Lajaunie, F. Boucher, R. Dessapt, P. Moreau, Strong anisotropic inﬂuence of local-ﬁeld effects on the dielectric response of α-MoO3, Phys. Rev. B 88 (2013) 115141. http://dx.doi.org/10.1103/PhysRevB.88.115141. [43] A.A. Bolzan, B.J. Kennedy, C.J. Howard, Neutron powder diffraction study of molybdenum and tungsten dioxides, Aust. J. Chem. 48 (1995) 1473–1477.

[44] J. Chen, J. Eng Jr, S. Kelty, NEXAFS determination of electronic and catalytic properties of transition metal carbides and nitrides: from single crystal surfaces to powder catalysts, Catal. Today 43 (1998) 147–158. [45] N. Jiang, J.C.H. Spence, Electron energy-loss spectroscopy of the OK edge of NbO2, MoO2, and WO2, Phys. Rev. B 70 (2004) 245117. http://dx.doi.org/ 10.1103/PhysRevB.70.245117. [46] G. Mountjoy, J. Yuan, P. Gaskell, Electron energy loss near edge spectroscopy of oxygen in amorphous and crystalline WO3 and MoO3, Inst. Phys. Conf. Ser., Boston: Adam Hilger, Ltd. (1993) 35–38 (c1985). [47] J. Purans, A. Kuzmin, P. Parent, C. Laffon, X-ray absorption study of the electronic structure of tungsten and molybdenum oxides on the OK-edge, Electrochim. Acta 46 (2001) 1973–1976. http://dx.doi.org/10.1016/S0013-4686(01) 00370-X. [48] P. Thakur, J.C. Cezar, N.B. Brookes, R.J. Choudhary, R. Prakash, D.M. Phase, et al., Direct observation of oxygen induced room temperature ferromagnetism in MoO2 thin ﬁlms by x-ray magnetic circular dichroism characterizations, Appl. Phys. Lett. 94 (2009) 062501. http://dx.doi.org/10.1063/1.3080679. [49] M. Sing, R. Neudert, H. Von Lips, M. Golden, M. Knupfer, J. Fink, et al., Electronic structure of metallic K0.3MoO3 and insulating MoO3 from high-energy spectroscopy, Phys. Rev. B. 60 (1999) 8559. [50] W. Luo, M. Varela, J. Tao, S.J. Pennycook, S.T. Pantelides, Electronic and crystalﬁeld effects in the ﬁne structure of electron energy-loss spectra of manganites, Phys. Rev. B 79 (2009) 052405. [51] J. Gaidelene, A. Kuzmin, J. Purans, Oxygen K-edge x-ray absorption near-edge structure in crystalline and amorphous molybdenum trioxides, J. Phys. Condens. Matter. 16 (2004) 6619–6625. http://dx.doi.org/10.1088/0953–8984/16/ 36/027. [52] J. Hwang, D. Kim, J.-S. Kang, S. Kolesnik, O. Chmaissem, J. Mais, et al., Soft x-ray absorption spectroscopy study of Mo-rich SrMn1 xMoxO3 (x⩾0.5), Phys. Rev. B 83 (2011) 073103. [53] G. Wu, T. Sekiguchi, Y. Baba, I. Shimoyama, X-ray absorption ﬁne structure and photon-stimulated ion desorption from solid MoO3 at molybdenum 3p 1/2, 3p 3/2 and oxygen 1 s edges, Nucl. Instrum. Methods Phys. Res. Sect. B: Beam Interact. Mater. At. 245 (2006) 406–410. [54] A.M. Arevalo-Lopez, M.A. Alario-Franco, Reliable method for determining the oxidation state in chromium oxides, Inorg. Chem. 48 (2009) 11843–11846. [55] T. Riedl, T. Gemming, W. Gruner, J. Acker, K. Wetzig, Determination of manganese valency in La1 xSrx MnO3 using ELNES in the (S)TEM, Micron 38 (2007) 224–230. http://dx.doi.org/10.1016/j.micron.2006.06.017. [56] S. Zhang, K.J. Livi, A.-C. Gaillot, A.T. Stone, D.R. Veblen, Determination of manganese valence states in (Mn3 þ , Mn4 þ) minerals by electron energy-loss spectroscopy, Am. Miner. 95 (2010) 1741–1746. [57] P. Potapov, D. Schryvers, Measuring the absolute position of EELS ionisation edges in a TEM, Ultramicroscopy 99 (2004) 73–85. [58] J. Scott, P. Thomas, M. MacKenzie, S. McFadzean, J. Wilbrink, A. Craven, et al., Near-simultaneous dual energy range EELS spectrum imaging, Ultramicroscopy 108 (2008) 1586–1594. [59] F. De Groot, Z. Hu, M. Lopez, G. Kaindl, F. Guillot, M. Tronc, Differences between L and L x-ray absorption spectra of transition metal compounds, J. Chem. Phys. 101 (1994) 6570. [60] R. Leapman, L. Grunes, P. Fejes, Study of the L23 edges in the 3d transition metals and their oxides by electron-energy-loss spectroscopy with comparisons to theory, Phys. Rev. B. 26 (1982) 614. [61] B. Thole, G. Van der Laan, Branching ratio in x-ray absorption spectroscopy, Phys. Rev. B 38 (1988) 3158. [62] K. Hirsch, V. Zamudio-Bayer, J. Rittmann, A. Langenberg, M. Vogel, T. Möller, et al., Initial-and ﬁnal-state effects on screening and branching ratio in 2p x-ray absorption of size-selected free 3d transition metal clusters, Phys. Rev. B 86 (2012) 165402. [63] R. Laskowski, P. Blaha, Understanding the L23 x-ray absorption spectra of early 3d transition elements, Phys. Rev. B. 82 (2010) 205104. [64] P. Krüger, Multichannel multiple scattering calculation of L23-edge spectra of TiO2 and SrTiO3: importance of multiplet coupling and band structure, Phys. Rev. B 81 (2010) 125121. [65] S. Nishida, S. Kobayashi, A. Kumamoto, H. Ikeno, T. Mizoguchi, I. Tanaka, et al., Effect of local coordination of Mn on Mn-L2,3 edge electron energy loss spectrum, J. Appl. Phys. 114 (2013) 054906.